# Optical properties

In document Carrier-Phonon Interaction in Semiconductor Quantum Dots (Page 148-166)

commutator in Eq. 7.16, which includes the instantaneous selfenergy contributions, reads

id

dt G<,cc(t) = Σδ,cc G<,cc−G<,ccΣδ,cc

+ Σδ,cvG<,vc−G<,cv Σδ,vc

(7.17a) id

dt G<,vv(t) = Σδ,vc G<,cv−G<,vcΣδ,cv

+ Σδ,vvG<,vv −G<,vvΣδ,vv

(7.17b) id

dt G<,cv(t) = Σδ,cc G<,cv −G<,ccΣδ,cv

+ Σδ,cvG<,vv−G<,cv Σδ,vv

(7.17c) id

dt G<,vc(t) = id

dt [G<,cv(t)] (7.17d)

with the band indices given explicitly. The lesser GFsG<,cvrepresent inter-band transition amplitudes that are diagonal and off-diagonal in the state index, i.e. direct and indirect inter-band transitions. On the other hand the intra-band quantities are given byG<,ccαβ and G<,vvαβ , describing the population forα = β and intra-band transition amplitudes forα = β. In Eq. (7.17), state and subband indices are still to be understood in matrix notation according to

Acc =

⎢⎢

νcνc νckc kcνc kckc

⎥⎥

⎦ , Acv =

⎢⎢

νcνv νck1v νckv2 νck1c kc1kv1 kc2kv2

⎥⎥

⎦ ,

Avc = [Acv] , Avv =

⎢⎢

⎢⎢

⎢⎢

⎢⎢

νvνv νvkv1 νvkv2 νvkv1 k1vk1v kv2k1v

νvkv2 k1vk2v kv2k2v

⎥⎥

⎥⎥

⎥⎥

⎥⎥

. (7.18)

Here, νλ indicates a QD state and knλ a WL state of the n-th subband, with λ represent-ing the correspondrepresent-ing band. In this example one conduction band and two subbands of the valence band are considered. Please note, that the QD states occur only once, even though the valence band contains two subbands. Furthermore the matrix notation implies a ”sum” over all states in the system. Depending on the sub-blocks of the matrices that are multiplied with each other in Eq. 7.17, this ”sum” is to be understood either as an integra-tion (2π)1 2

d2kover a continuum of WL states or a summation

R,ν over QD states and positions.

Instantaneous selfenergy contributions

As instantaneous selfenergy contributions we consider in the following the free-particle energy dispersion, the optical pulse excitation, and Coulomb renormalizations in SX-CH approximation. A detailed discussion of the different selfenergy contributions is presented in Chap. 4. Consequently, only a short summary is given, where nitride-speciﬁc properties are discussed.

The energy dispersionελα we consider for the calculation is depicted in Fig. 7.10 and in-cluded by means of the selfenergy

Σfreeαβ,λλλαδαβ δλλ . (7.19) Off-diagonal dipole transitions are driven by the optical pulse, which is included via the selfenergy (4.50). Only those transition amplitudesG<,cvαβ are driven whose corresponding dipole matrix elementsdcvαβ are nonzero. For InGaAs QDs the selfenergyΣδ = Σfreepulse is diagonal in the state index. In this case no off-diagonal elements of G<αβ are driven in the SBE (7.16), even in the presence of two valence bands. For InN QDs where also the off-diagonal dipole coupling for the QD states is taken into account, the corresponding interband transition amplitudes G<,cv are driven by the pulse directly. Other inter- and intra-band transition amplitudes can be driven indirectly, for example via the Coulomb interaction.

The Coulomb interaction is considered by means of the SX-CH selfenergy (4.19) and (4.20), as well as the Hartree contributions (4.12). To facilitate the discussion of off-diagonal contributions, let us ﬁrst focus on the diagrammatic representation of the Hartree terms is depicted in Fig. 4.3b. As we are restricting ourselves to interaction vertices diag-onal in the band index, only population functions3 appear in the Hartree terms. Were we to include all possible band-index combinations in the overlaps, also Hartree contributions containing interband transition amplitudes would appear. The corresponding diagrammatic representation for the SX-CH selfenergy is depicted in Fig. 4.3a. Due to the off-diagonal nature of the main QD transitions, cf. the dipole selection rules, the selfenergy for the WL states reads

Σλλkk(t) = i

νμ

Vkνkμλλ G<,λλμν (t) + i

k

VkkλλkkG<,λλkk(t), (7.20) where all GFs G<,cvδγ involving two QD states are non-vanishing and hence all interaction matrix elementsVkγkδλλ are required. As the WL-WL overlaps (7.14) contain the momentum conservation, we can restrict our analysis to diagonal WL GFsGkk. Note, that inVkkλλkk

we have to deal with the problem of lifting the Coulomb singularity. The procedure we

3In principle also intra-band transitions amplitudes.

use is discussed in Refs. [64] and an extension to the TB approach is outlined in App. B.4.

Likewise we ﬁnd for the QD states Σλλνμ(t) = i

k

Vνkμkλλ G<,λλkk (t) + i

χξ

Vνχμξλλ G<,λλξχ (t), (7.21) where all QD-QD couplingsVνχμξλλ are included.

The complicated interplay of all transition amplitudes via the Coulomb matrix elements poses the question, whether transition amplitudes that are not directly driven by the optical ﬁeld via the dipole interaction can be driven indirectly via the Coulomb interaction. To in-vestigate this, let us consider for example the dynamics of a interband transition amplitude connecting QD and WL statesG<,cvνk . The corresponding equation of motion for this GF reads

id

dtGcvνk(t) = i

+ ΣccνkGcvkk+ ΣcvνkGvvkk + ΣccννGcvνk+ ΣcvννGvvνk

−GccνkΣcvkk−GcvνkΣvvkk

−GccννΣcvνk−GcvννΣvvνk

, (7.22)

where the indices k and ν are to be understood symbolically for the respective state be-longing either to the WL or to a QD. Furthermore the≷ components are suppressed for simplicity. All contributions that drive this polarization are proportional to a polarization times a population. Therefore, in the linear regime, i.e. χ(1), these terms are not driven in the limit of vanishing background carrier density. Considering ﬁnite background carrier densities, e.g. for gain calculations, these terms in principle have to be taken into account.

However, all transition amplitudes not directly driven by the optical pulse, i.e.dαβ = 0, do not directly contribute to the macroscopic polarization (6.5). Their inﬂuence is restricted to the back-action on directly driven polarizations. To simplify the numerical evaluation, we therefore neglect these transition amplitudes in the following. Similar to the discussion for the Hartree terms, the inclusion of band off-diagonal vertices implies additional terms.

### 7.4.2 Linear absorption

The linear absorption spectrum is calculated from the macroscopic polarization viaχ(ω) =

P(ω)E(ω) ∝ α(ω)as discussed in Chap. 6.1. As the SX-CH and the Hartree selfenergies we consider for the calculation do not provide microscopic dephasing, in a ﬁrst step we use a phenomenological value of γ =10 meV. Calculations that additionally include micro-scopic dephasing due to carrier-LO-phonon collisions are presented below. In comparison to typical InGaAs QDs discussed in previous chapters, the InN QD under consideration exhibits deeply conﬁned shells, especially for electrons, cf. Fig. 7.10. The conﬁnement

energy for the lowest QD states with respect to the band edge is -575.4 meV and -345.3 meV for electrons, and -49.6 meV and -39.8 meV for holes. In conjunction with the ”skew”

dipole selection rules discussed in Chap. 7.2.5, this corresponds to free-carrier transition energies of -615.2 meV and -394.9 meV, relative to the WL bandgap of 1731 meV. As initial carrier distribution, we assume a quasi-equilibrium situation for the CB as well as a common one for the two VBs.

1000 1200 1400 1600

energy in meV 0

2 4 6 8 10

absorption in arb. units

7.0e09 cm-2 1.2e10 1.7e10 2.0e10 5.0e10 2.0e11

Fig. 7.15: Linear optical absorption spectra for InN QDs at 300 K and for various carrier densities, considering a phenomenological dephasing of 10 meV.

The corresponding absorption spectra for a temperature of 300 K and various carrier densi-ties are shown in Fig. 7.15. With increasing carrier density, the transition energies exhibit a blue shift accompanied by bleaching of the absorption and transition to gain. For carrier densities exceeding 5×1010cm−2 the blue shift is reduced. This complicated behavior is due to the interplay of Hartree, screened-exchange (SX) and Coulomb hole (CH) con-tributions. The corresponding numbers for three exemplary carrier densities are given in Tab. 7.2. As we can infer, the CH energy shifts are practically the same for CB and VB carriers and therefore only slightly inﬂuence the interband transition energies. In contrast, Hartree as well as SX terms give rise to a relative shift of CB and VB energies. Since for each band the Hartree term contains contributions from all bands (cf. Eq. (4.12) and Fig. 4.3b), the inﬂuence of the QD population on the Hartree shift is similar for CB and VB. The large difference between CB and VB shifts arises from the screened interaction matrix elements. The blue shift for small to intermediate carrier densities stems from the steep increase of the Hartree contributions. For larger carrier densities, the Hartree terms saturate due to ﬁlling of the QD states. Simultaneously the screening of the Coulomb

2×1010cm−2 5×1010cm−2 2×1011cm−2

CB SX 1 -73.7 -88.9 -64.5

SX 2 -17.5 -58.3 -46.3

CH 1 -14.1 -20.1 -36.5

CH 2 -13.3 -18.6 -31.9

H 1 149.0 285.5 189.4

H 2 124.8 245.7 156.2

VB SX 1 2.9 6.4 15.4

SX 2 2.4 5.4 14.4

CH 1 -13.9 -19.7 -35.6

CH 2 -14.0 -19.9 -36.3

H 1 -13.3 -29.1 -70.1

H 2 -14.4 -31.7 -79.1

Tab. 7.2: Energy shift contributions from screened-exchange (SX), Coulomb hole (CH), and Hartree (H) selfenergies in meV.

interaction increases due to ﬁlling of WL states which leads to a strong reduction of the Hartree contributions. In contrast, saturation effects are smaller for the SX terms because of increasing contributions from WL carriers. This leads in total to a reduced blue shift for high carrier densities.

To employ a microscopic dephasing mechanism we consider the interaction with LO phonons, where, similar to the extended discussion in Chap. 5.2.2, we use the RPA selfen-ergy. Speciﬁcally, we consider the one-time collision terms (3.72) in the Markovian limit which is obtained by application of the reverse GKBA, cf. Chap. 3.5. This procedure

yields d

dtG<,cvαβ (t)

coll = 2

γδξ

q

t

−∞

dt3

+ Gcc,>δξ (t)Gc,ξR(t, t3)Dαξγδ,qcccc,<(t3, t)Gc,γA(t3, t)Gcv,<γβ (t)

− Gcc,<δξ (t)Gc,ξR(t, t3)Dcccc,>αξγδ,q(t3, t)Gc,Aγ (t3, t)Gcv,>γβ (t) + Gcc,<αγ (t)Gc,Rγ (t, t3)Gc,Aδ (t3, t)Gcv,>δξ (t)Dγξβδ,qcvvc,<(t, t3)

− Gcc,>αγ (t)Gc,γR(t, t3)Gc,δA(t3, t)Gcv,<δξ (t)Dγξβδ,qcvvc,>(t, t3) + Gcv,>δξ (t)Gv,ξR(t, t3)Dcvvc,<αξγδ,q(t3, t)Gv,γA(t3, t)Gvv,<γβ (t)

− Gcv,<δξ (t)Gv,ξR(t, t3)Dcvvc,>αξγδ,q(t3, t)Gv,Aγ (t3, t)Gvv,>γβ (t) + Gcv,<αγ (t)Gv,Rγ (t, t3)Gv,δA(t3, t)Gvv,>δξ (t)Dγξβδ,qvvvv,<(t, t3)

− Gcv,>αγ (t)Gv,γR(t, t3)Gv,δA(t3, t)Gvv,<δξ (t)Dvvvv,>γξβδ,q(t, t3) . (7.23) withDαβγδ(t1, t2)containing the interaction matrix elements as well as the phonon propa-gator, cf. Eq. 4.32. Also in this case a separation into diagonal and off-diagonal dephasing is possible, even though the situation is more complicated due to the coupling of different off-diagonal GFs. Nevertheless, a compensation between the two contributions also holds in this case.

The corresponding optical absorption spectra including dephasing due to LO-phonon col-lisions are presented in Fig. 7.16. Energy shifts due to polaron effects are small in compar-ison to SX-CH and Hartree interaction which are identical as in the results shown above.

The main inﬂuence of carrier-phonon scattering is dephasing of the optical polarization that corresponds to broadening of the resonances. An asymmetric line shape as well as a typical line width of 22 meV for the energetically lower and 18 meV for the energetically higher transition are found. The difference arises due to the fact that for the energetically lower transition the off-diagonal compensation is reduced due to the large energetic sepa-ration from the WL. It should be noted, that at the low energy side of the QD resonances a slightly negative absorption is observed. This artifact we attribute to the GKBA, since as shown in Chap. 5.3.3 the validity of the GKBA for intermediate to strong polar coupling materials is questioned.

1000 1200 1400 1600 energy in meV

0 2 4 6 8 10

absorption in arb. units

7.0e09 cm-2 1.2e10 1.7e10 2.0e10 5.0e10 2.0e11

Fig. 7.16: Linear optical absorption spectra for InN QDs at 300 K and for various carrier densities. The dephasing is provided by carrier-LO-phonon collisions and included on a microscopic basis.

### 7.4.3 Dephasing due to Coulomb scattering

Absorption spectra for InGaAs QDs are presented in Chap. 6.1. To determine excitation-induced dephasing due to Coulomb interaction the second Born approximation (SBA) was employed, cf. Chap. 4.1. In contrast, for the nitride material system we use the SX-CH approximation. Therefore several comments on important differences between the two approaches are in order.

t1 t1 t1

(a) SX-CH

t1 t2 t1

(b) direct SBA

t1 t2 t1

(c) exchange SBA

Fig. 7.17: Schematic representation of SX-CH diagrams SBA diagrams.

Schematically, the contributing diagrams in the Kadanoff-Baym equations (3.64) are de-picted in Fig. 7.17. In contrast to the usual notation, the wiggly interaction line denotes the retarded/advanced plasmon GFWR/A and the carrier propagators Gare represented by

straight lines. Therefore, these diagrams should not be confused with Feynman diagrams as no systematic perturbation expansion is implied. For the following discussion note, that WR/A is a real quantity under the assumption that the screening is instantaneous and does not contain retardation effect, cf. the discussion in Chap. A.2. Considering the homoge-neous part of the equation of motion for the polarization, idt = Δψ, the dephasing is identiﬁed as the imaginary part ofΔ. In the SX-CH selfenergy diagram (cf. Fig. 7.17a) no retardation effects are included due to the instantaneous interaction and hence all internal times are ﬁxed to the external ones. This implies the structureΔ∝WR/Af, which is a real quantity and hence provides no dephasing. In contrast, in the SBA diagrams an internal time t2 is involved (cf. Fig. 7.17b,c). Hence, retardation effects, that are included in the two-time propagatorsG(t1, t2), contribute. This can be easily seen when representing the two-time propagator by means of the GKBA, which maps the two-time propagators onto the time-diagonal with the help of retarded/advanced GFs, cf. Chap. 3.5. For the equation of motion this implies the structureΔ =W Wf f f GRGRGRGR, which is complex in gen-eral, and hence provides dephasing. However, the inclusion of dephasing due to Coulomb scattering in our calculations for nitride semiconductors remains a challenging task as in addition to the calculations shown in Chap. 6.1 one has to account for off-diagonal GFs.

Moreover, in the calculations for the InGaAs material using the harmonic-oscillator model (cf. Chap. A.1) the matrix elements to a large extend can be calculated analytically, which is not possible in the nitride case and thus by far enhancing the computational effort.

This thesis provides a deeper insight into to carrier-LO-phonon scattering mechanism in semiconductor QDs. On the one hand the interaction gives rise to renormalizations of the single-particle states, and on the other hand it leads to carrier scattering and dephasing processes. The interplay of these two effects was studied using the framework of non-equilibrium Green’s functions.

Most important for the understanding of scattering and dephasing mechanism are the renor-malizations of the single-particle states. In case of the carrier-LO-phonon interaction, they are described by the formation of polarons. An intuitive approach for the discussion of polarons is the spectral function, which is connected to the density of states. For con-tinuous systems like QWs, the spectral function is dominated by a single resonance. In this case results from perturbation theory are in good agreement with our non-perturbative approach, leading simply to a shift of the free-particle energies and introducing a ﬁnite carrier lifetime. In contrast, for QD systems perturbation theory clearly fails. The carrier conﬁnement gives rise to an enhanced effective coupling, resulting in pronounced phonon satellites and their hybridization. Strong coupling effects are observed, even for weak polar coupling materials. Additionally, the interaction of QD states with the energetically close continuum of WL states leads to a further broadening of the polaron resonances at room temperature. In contrast, at low temperatures only a few phonons are present. As a con-sequence, phonon absorption processes are strongly suppressed and emission processes dominate. This leads to a much weaker interaction between QD and WL states, resulting in much narrower resonances of the spectral function.

These polaron properties determine to a large extent the efﬁciency of carrier-scattering processes, as the scattering kernel is given by the overlap of the spectral functions of the involved states. Thus, within the quasi-particle picture of carrier-scattering a deeper in-sight into the phonon-bottleneck controversy was achieved. Because of the controversial experimental ﬁndings regarding the phonon-bottleneck discussion, further investigations have been performed. For elevated temperatures we ﬁnd that polaron effects give rise to fast scattering channels, whereas in the low-temperature regime an initial fast relaxation is followed by a freezing of the carrier distribution at later times, not reaching a thermal dis-tribution. Thus, our analysis shows that the phonon bottleneck discussion in QDs should include the energy spectrum of the QD, the temperature regime, and the timescales in-volved. The question about the presence of a phonon bottleneck can not be answered by the energy mismatch argument alone. As applications of the developed quantum-kinetic

model we have presented an investigation of the inﬂuence of carrier-phonon scattering on the optical response by means of absorption spectra and the temporally resolved photolu-minescence. The analysis of the optical response, including dephasing processes due to both, carrier-carrier and carrier-phonon interaction, showed that it is essential to consider quasi-particle renormalizations in a self-consistent way. Furthermore it was found that both contributions to the dephasing are important, even in the high carrier-density regime.

For the nitride material system it turned out that, besides many-body effects, a micro-scopic treatment of the electronic properties is of central importance, as intrinsic and strain-induced electric ﬁelds as well as the QD geometry and the underlying wurtzite crystal structure strongly inﬂuence the electronic properties. To study the interplay of the par-ticular single-particle wave functions and many-body effects, a procedure to incorporate results from an atomistic tight-binding approach into our quantum-kinetic theory was de-veloped. As a ﬁrst application the properties of nitride polarons have been investigated. In a second step absorption spectra are presented where we considered Coulomb renormaliza-tions as well as the dephasing due to carrier-phonon interaction including polaron effects.

These results show large excitation-induced shifts of the QD resonances, which deﬁnitely have to be considered for practical applications like LEDs and laser diodes.

### Future directions

The results presented in this thesis may serve as a starting point for further investigations in the ﬁeld of quantum kinetics and semiconductor quantum dot systems. Whereas the one-time kinetics provides an intuitive way to incorporate memory effects and quasi-particle renormalizations, intrinsic shortcomings of the involved GKBA, in particular for interme-diate to strong polar coupling materials, should be investigated further. Such investigations might for example include new quasi-particle concepts presented by Velický et al. [89], a more detailed analysis of the reconstruction scheme for two-time propagators, and a further analysis of the two-time equations including the kinetics of individual polaron satellites.

For the carrier scattering a calculation of the temporal evolution of the population distri-bution including both, carrier-carrier and carrier-phonon interaction, would be interesting, especially since the relaxation times we computed indicate that in QD systems even at low carrier densities Coulomb scattering is not negligible. With the new generation of CPU clusters such calculations in a one-time version should be feasible. Another aspect for the optical response of semiconductor QDs is the exciton phonon interaction, represented by selfenergy diagrams that contain both carrier-carrier and carrier-phonon interaction lines.

Such contributions, giving rise to phonon replica of the exciton resonances in the optical spectra, are clearly observed in experimental data. Furthermore, the procedure presented to incorporate wave functions obtained from atomistic tight-binding calculations opens a whole ﬁeld of future investigations. For the nitride material system, especially the inﬂu-ence of speciﬁc material compositions, e.g. ternary alloys, concentration gradients due to

tions, QD geometry and strain, obtained for example with a transmission-electron micro-scope. Using these data as input for a tight-binding calculation, immediately enables us to determine the optical response including many-body effects.

### A.1 Envelope wave function model

Based on the symmetry properties of the QD-WL system, one assumes for the wave func-tions in Bloch representation a factorization of the envelope function into an 2D in-plane partϕ(ρ)and an 1D partξ(z)in growth direction,

ψ(r) =ϕ(ρ)ξ(z)uk≈0(r), (A.1)

with the lattice periodic Bloch functionuk≈0(r). The envelope part in growth direction is described by a 1D quantum well (QW) wave function, where only the lowest subband is taken into account. The simplest approach would be to consider QW barriers of inﬁnite height, where the eigenfunctions are known analytically, ξ(z) = sin-π

Lz.

. Considering barriers of ﬁnite height or a more complicated potential to incorporate e.g. the Quantum conﬁned Stark effect (see Chap. 7.1), the envelope part is evaluated numerically by dis-cretization of the corresponding 1D Schrödinger equation in real space, see e.g. [202, 203].

In the absence of QDs, the delocalized states are described by 2D plane waves (PW)

ϕ0k() = √1

A eik, (A.2)

withkbeing the 2D in-plane momentum. Considering ﬂat, lens-shaped quantum dots, the in-plane conﬁnement potential was shown to be harmonic in good approximation [140, 204]. The corresponding 2D harmonic oscillator wave functions are well known [29] and classiﬁed by their angular momentum properties. Correspondingly they are referred to as

s-, p- and d-shell.

ϕsm=0(−R) = β

√π eβ

2|−R|2

2 , (A.3a)

ϕpm=±1(−R) = β

√π eβ

2|−R|2

2 ·β|−R|e±iφ, (A.3b)

ϕdm=±2(−R) = β

√π eβ

2|−R|2

2 · (β |−R|)2 e±i2φ, (A.3c) ϕdm=0(−R) = β

√π eβ2|−R|2 2 · (β(−R|)2−1

(A.3d) In this notation R is the position of the QD on the WL plane and β = mΔE is the inverse oscillator length, determining the equidistant energy separationΔE between the QD shells.

### Interaction matrix elements

According to the separation ansatz (A.1), thez-dependence in the bare Coulomb interac-tion matrix elements (4.1) might be cast into a formfactor,

V1234 = e2 4πε0

d2q 1

q F1234(q) φ1|eiqρ4 φ2|e−iqρ3 (A.4) with

F1234(q) =

dz

dz ξ(z)ξ(z)eiqz (z−z)ξ(z)ξ(z). (A.5) The overlap integrals for the QD-WL system under consideration are discussed below.

Note, that the Carrier-LO-phonon interaction matrix elements and the bare Coulomb inter-action matrix elements are connected according to (4.37).

### Orthogonalized plane waves

As for the in-plane part the harmonic oscillator states and the plane waves are orthogo-nal among themselves but not among each other, the orthogoorthogo-nalized-plane-waves (OPW) scheme is applied,

|k= 1 Nk

|k0

ν,R

|ν,R ν,R|k0

, (A.6)

Nk =

1−N

ν

| k0|ν |2 . (A.7)

Here, explicitly the random distribution of QDs on the WL plane was used. Since the QD position only gives rise to a phase factor ν,R|k0 = ν|k0 eikR, on average momen-tum conservation is restored, k|k ∝ δ(k −k). Keeping in mind that k0|ν ∝ 1A, effectively only the QD densityNQD = NA enters the theory.

In principle the OPW scheme also leads to a modiﬁcation of the energies of the WL states.

However, this change can be neglected if the QD density and the QD size are sufﬁciently small or, in other words, if the fraction of the WL plane that is covered with QDs is sufﬁ-ciently small. Consider the expectation value of the total energy for the total Hamiltonian containing QD and WL states,

k|H|k=k0|H|k0 −N

ν

k0|H|ν ν|k0 −N

ν

k0|ν ν|H|k0

+N

ν,μ

k0|ν ν|H|μ μ|k0

=k0|H|k0 −N

ν

Eν| ν|k0 |2 . (A.8)

Taking into account that the overlaps| ν|k0 |2contain factors of A1, we ﬁnd that in the last line the second term is proportional to the QD densityNQD. This shows that for sufﬁciently low QD densities (in the sense explained above), we can disregard the OPW corrections to the WL energies. As the WL energies in the presence of QDs are not known, we work in good approximation work with the PW energiesk0|H|k0 ≈Ek0. However, as the matrix elements calculated from non-orthogonal states lead to clear deviations in the results, it is essential to include the OPW corrections to the wave-functions.

### Overlap integrals

For the calculation of Coulomb and Fröhlich interaction matrix elements, see Chap. 4, overlap integrals of the formα|eiqr|βhave to be evaluated. Using the OPW scheme and assuming identical QDs, we ﬁnd for the QD-WL overlaps

ν|eiqr|k= 1 Nk

ν|eiqr|k0

ν

ν|eiqr ν|k0

, (A.9)

and for the WL-WL overlaps

k|eiqr|k=δ(q+kk)DOPW(k,q,k), (A.10)

In document Carrier-Phonon Interaction in Semiconductor Quantum Dots (Page 148-166)